en sv fi en en en en ru cs da ar es sv ro el fa fr nl hu tr zh de pl fi vi ko it hbs_lat da th ja pt da da da sv de da fi en de sv da sv en da da da da da da eo da en da de eo en sv en en fr en en en en en en en es da it da en en es da en en da da en sv en en da da nl da da da it it da da da da nl pl en nl de en en en en en en en en en en en ca en en en en en en en en en en en en en en en en en en en en en en en en en en en en en da da da da da da da en da en en en en en en en en en en en da da da da da da en fr da
High Strength Low Alloy V Steels: Part One :: Total Materia Article
Institutter og den akademiske verden
Deep Drawable Steels: Part One
Thermo-Mechanical Treatment (TMT) of Non-Ferrous Alloys: Part One
DataPLUS er et supplerende data modul som leverer korrosions data, materiale samlings information, materiale dimensioner og tolerancer og belægnings informationer for tusinder af metalliske og ikke-metalliske materialer.
Klik her for at se mere.
Overview of Total Materia database 12th January 2022
Total Materia har ved at give os en bestemt metode tilladt os at løse alle problemerne vi havde med søgning af alternative materialer i udlandet. Takket være Total Materia har vi udstedt virkelige "internationale" specifikationer for køb af stål i fremmede lande.
Total Materia er fortsat det eneste værktøj, der vil blive brugt til dette formål.
Bonfiglioli Industrial Gearmotors, Bologna, Italia
Vores mission er simpel;
at gøre Total Materia
til det eneste destination og
første valg for ingeniører
Prof. Dr. Viktor Pocajt, CEO
Key to Metals AG
High Strength Low Alloy V Steels: Part One
High-strength low-alloy (HSLA) steels, or microalloyed steels, are designed to provide better mechanical properties and/or greater resistance to atmospheric corrosion than conventional carbon steels.
Vanadium contributes to strengthening by forming fine precipitate particles (5 to 100 nm in diameter) of V(CN) in ferrite during cooling after hot rolling.
Low alloy steel is one of te most rapidly developed and highly utilized steel grades in recent years and has become te most produced, applied and economic steel available. Te stipulated minimum yield strength is 275 MPa with a maximum value of 1035 MPa. A category of steel with these characteristics is made by adding a small proportion of alloy element in te carbon steel, which will ensure te steel has high strength, good toughness, high weldability and strong formality and erosion resistance under hot rolling or heat treatment conditions.
Normal elements for alloyment are generally strong carbide combination elements such as Ti, Nb and V. Nb are most widely applied and are te subject of most research projects due to te fact that it can effectively condition various physical metallurgy factors and have te biggest refinement and precipitation strengthening in traditional controlled rolling process. However, there has never been an equal determination to study te research and development of Ti-alloyed and V-alloyed microstructural steels.
High-strength low-alloy (HSLA) steels, or microalloyed steels, are designed to provide better mechanical properties and/or greater resistance to atmospheric corrosion than conventional carbon steels. They are not considered to be alloy steels in te normal sense because they are designed to meet specific mechanical properties rather than a chemical composition (HSLA steels have yield strengths greater than 275 MPa, or 40 ksi). Te chemical composition of a specific HSLA steel may vary for different product thicknesses to meet mechanical property requirements.
Te HSLA steels in sheet or plate form have low carbon content (0.05 to −0.25% C) in order to produce adequate formability and weldability, and they have manganese content up to 2.0%. Small quantities of chromium, nickel, molybdenum, copper, nitrogen, vanadium, niobium, titanium, and zirconium are used in various combinations.
Niobium and vanadium, te most frequently used micro alloy additives, are added to achieve similar objectives-to condition te austenite and to precipitate at various stages of processing. These two elements are not interchangeable however, and for optimum results, specific steel chemistry and processing parameters are required.
Solubility of M (C,N) in austenite
Propensity for Concast Cracking
N effect on Precipitation in austenite
N effect on Precipitation in ferrite
Table 1: Critical size of macro inclusions in cast semis that cause process upsets and product defects
High strength low alloy (HSLA) steels offer te advantage of weight and cost savings compared to mild steel. Therefore they are widely used in te automotive and te construction industry.
Te development of vanadium containing steels occurred shortly after te development of weathering steels, and flat-rolled products. With up to 0.10% V these materials are widely used in a hot-rolled condition. Vanadium-containing steels are also used in te controlled-rolled, normalized, or quenched and tempered condition.
Vanadium contributes to strengthening by forming fine precipitate particles (5 to 100 nm in diameter) of V(CN) in ferrite during cooling after hot rolling. These vanadium precipitates, which are not as stable as niobium precipitates, are in solution at all normal rolling temperatures and thus are very dependent on te cooling rate for their formation. Niobium precipitates, however, are stable at higher temperatures, which is beneficial for achieving fine-grain ferrite.
Te austenite grain size of hot-rolled steels is determined by te recrystallization and grain growth of austenite during rolling. Vanadium hot-rolled steels usually undergo conventional rolling but are also produced by recrystallization controlled rolling. With conventional rolling, vanadium steels provide moderate precipitation strengthening and relatively little strengthening from grain refinement. Te maximum yield strength of conventionally hot-rolled vanadium steels with 0.25% C and 0.08% V is about 450 MPa (65 ksi). Te practical limit of yield strengths for hot-rolled vanadium-microalloyed steel is about 415 MPa (60 ksi), even when controlled rolling techniques are used.
Vanadium steels subjected to recrystallization controlled rolling require a titanium addition so that a fine precipitate of TiN is formed that restricts austenite grain growth after recrystallization. Yield strengths from conventional controlled rolling are limited to a practical limit of about 415 MPa (60 ksi) because of te lack of retardation of recrystallization. When both strength and impact toughness are important factors, controlled-rolled low-carbon niobium steel (such as X-60 hydrogen-induced cracking resistant plate) is preferable.
Skriv en sætning for at søge efter:
Denne artikel tilhører en serie af artikler. Du kan klikke på linkene nedenfor for at læse mere om dette emne.
High Strength Low Alloy V Steels: Part Two
High Strength Low Alloy V Steels: Part Three
Finding chemical composition data in te Total Materia database
Finding chemical composition data in te Total Materia database couldn’t be easier.
Within seconds it is possible for you to find useful chemical composition data for over 175,000 materials in te database.
Enter te material of interest into te quick search field. You can optionally narrow your search by specifying te country/standard of choice in te designated field and click Search.
Total Materia will generate te search list for you to select te material of interest from te material list.
Click on te material of interest.
On te subgroup page, click te composition link to view chemical composition data for te selected material. Te number of chemical composition data records is displayed in brackets next to te link.
Te chemical composition data will be then be displayed along with all selected material information for your reference.
For you’re a chance to take a test drive of te Total Materia database, we invite you to join a community of over 150,000 registered users through te Total Materia Free Demo.
© 2022 Key to Metals AG. Alle Rettigheder Forbeholdes